DOI: 10.17188/1718656
title: Materials Data on BaCa3Zr16(PO4)24 by Materials Project

description: BaCa3Zr16(PO4)24 crystallizes in the triclinic P-1 space group. The structure is three-dimensional. Ba is bonded in a distorted hexagonal planar geometry to six O atoms. All Ba–O bond lengths are 2.67 Å. There are two inequivalent Ca sites. In the first Ca site, Ca is bonded in a distorted hexagonal planar geometry to six O atoms. There are one shorter (2.50 Å) and five longer (2.51 Å) Ca–O bond lengths. In the second Ca site, Ca is bonded in a distorted hexagonal planar geometry to six O atoms. There are four shorter (2.50 Å) and two longer (2.51 Å) Ca–O bond lengths. There are eight inequivalent Zr sites. In the first Zr site, Zr is bonded to six O atoms to form ZrO6 octahedra that share corners with six PO4 tetrahedra. There are three shorter (2.04 Å) and three longer (2.16 Å) Zr–O bond lengths. In the second Zr site, Zr is bonded to six O atoms to form ZrO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Zr–O bond distances ranging from 2.03–2.19 Å. In the third Zr site, Zr is bonded to six O atoms to form ZrO6 octahedra that share corners with six PO4 tetrahedra. There are three shorter (2.05 Å) and three longer (2.19 Å) Zr–O bond lengths. In the fourth Zr site, Zr is bonded to six O atoms to form ZrO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Zr–O bond distances ranging from 2.03–2.19 Å. In the fifth Zr site, Zr is bonded to six O atoms to form ZrO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Zr–O bond distances ranging from 2.07–2.12 Å. In the sixth Zr site, Zr is bonded to six O atoms to form ZrO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Zr–O bond distances ranging from 2.07–2.13 Å. In the seventh Zr site, Zr is bonded to six O atoms to form ZrO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Zr–O bond distances ranging from 2.08–2.16 Å. In the eighth Zr site, Zr is bonded to six O atoms to form ZrO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of Zr–O bond distances ranging from 2.07–2.15 Å. There are twelve inequivalent P sites. In the first P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with four ZrO6 octahedra. The corner-sharing octahedra tilt angles range from 24–42°. There are a spread of P–O bond distances ranging from 1.54–1.56 Å. In the second P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with four ZrO6 octahedra. The corner-sharing octahedra tilt angles range from 25–41°. There are a spread of P–O bond distances ranging from 1.54–1.56 Å. In the third P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with four ZrO6 octahedra. The corner-sharing octahedra tilt angles range from 24–42°. There are a spread of P–O bond distances ranging from 1.54–1.56 Å. In the fourth P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with four ZrO6 octahedra. The corner-sharing octahedra tilt angles range from 23–34°. There is two shorter (1.54 Å) and two longer (1.55 Å) P–O bond length. In the fifth P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with four ZrO6 octahedra. The corner-sharing octahedra tilt angles range from 25–41°. There are a spread of P–O bond distances ranging from 1.54–1.56 Å. In the sixth P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with four ZrO6 octahedra. The corner-sharing octahedra tilt angles range from 24–41°. There are a spread of P–O bond distances ranging from 1.54–1.56 Å. In the seventh P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with four ZrO6 octahedra. The corner-sharing octahedra tilt angles range from 24–41°. There are a spread of P–O bond distances ranging from 1.54–1.56 Å. In the eighth P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with four ZrO6 octahedra. The corner-sharing octahedra tilt angles range from 22–35°. There is three shorter (1.54 Å) and one longer (1.55 Å) P–O bond length. In the ninth P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with four ZrO6 octahedra. The corner-sharing octahedra tilt angles range from 24–42°. There are a spread of P–O bond distances ranging from 1.54–1.56 Å. In the tenth P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with four ZrO6 octahedra. The corner-sharing octahedra tilt angles range from 25–41°. There are a spread of P–O bond distances ranging from 1.54–1.56 Å. In the eleventh P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with four ZrO6 octahedra. The corner-sharing octahedra tilt angles range from 22–35°. There are a spread of P–O bond distances ranging from 1.53–1.55 Å. In the twelfth P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with four ZrO6 octahedra. The corner-sharing octahedra tilt angles range from 24–42°. There are a spread of P–O bond distances ranging from 1.54–1.56 Å. There are forty-eight inequivalent O sites. In the first O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the second O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the third O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the fourth O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the fifth O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the sixth O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the seventh O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the eighth O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the ninth O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the tenth O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the eleventh O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the twelfth O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the thirteenth O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the fourteenth O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the fifteenth O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the sixteenth O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the seventeenth O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the eighteenth O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the nineteenth O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the twentieth O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the twenty-first O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the twenty-second O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the twenty-third O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the twenty-fourth O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the twenty-fifth O site, O is bonded in a 3-coordinate geometry to one Ca, one Zr, and one P atom. In the twenty-sixth O site, O is bonded in a 3-coordinate geometry to one Ba, one Zr, and one P atom. In the twenty-seventh O site, O is bonded in a 3-coordinate geometry to one Ca, one Zr, and one P atom. In the twenty-eighth O site, O is bonded in a 3-coordinate geometry to one Ca, one Zr, and one P atom. In the twenty-ninth O site, O is bonded in a 3-coordinate geometry to one Ca, one Zr, and one P atom. In the thirtieth O site, O is bonded in a 3-coordinate geometry to one Ba, one Zr, and one P atom. In the thirty-first O site, O is bonded in a 3-coordinate geometry to one Ca, one Zr, and one P atom. In the thirty-second O site, O is bonded in a 3-coordinate geometry to one Ca, one Zr, and one P atom. In the thirty-third O site, O is bonded in a 3-coordinate geometry to one Ba, one Zr, and one P atom. In the thirty-fourth O site, O is bonded in a 3-coordinate geometry to one Ca, one Zr, and one P atom. In the thirty-fifth O site, O is bonded in a 3-coordinate geometry to one Ca, one Zr, and one P atom. In the thirty-sixth O site, O is bonded in a 3-coordinate geometry to one Ca, one Zr, and one P atom. In the thirty-seventh O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the thirty-eighth O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the thirty-ninth O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the fortieth O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the forty-first O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the forty-second O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the forty-third O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the forty-fourth O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the forty-fifth O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the forty-sixth O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the forty-seventh O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom. In the forty-eighth O site, O is bonded in a bent 150 degrees geometry to one Zr and one P atom.